Scantling and rolling tolerances have been progressively optimised and the ability of coatings to resist
corrosion over extended periods is the crucial factor in safeguarding the capital investment locked up in the
structure of the vessel.
Understanding how coatings reduce corrosion rates and how coatings eventually breakdown and must be
replaced is an essential part of safe vessel operation. This chapter deals with the basic theory of corrosion and
sets out the various factors controlling breakdown rates.
Corrosion of steel in ballast and cargo tanks may be defined as an electrochemical process in which the steel
reacts with its environment to form an oxide, or other compound, similar to the ore from which it was
The majority of metals are found in nature in the mineral state, that is, in their stable oxidised condition as
oxides, chlorides, carbonates, sulphates, sulphides, etc. The extraction of a metal from the mineral involves a
reduction process, which requires a great deal of energy. As a consequence of this large energy input the
metal is in a high-energy condition and will endeavour to return to its former stable oxidised low Energy State,
as quickly as environmental conditions will allow. It is this energy difference between the pure metal and its
oxidised forms which is the driving force for corrosion of the metal. Many corrosion products show a chemical
similarity to the corresponding minerals. Iron, for example, is extracted from its ores, mainly oxide and
carbonate, by reduction with carbon in a blast furnace. In the presence of moisture and oxygen, the iron metal
so obtained is oxidised to rust, which is chemically the same as its ore.
Uncoated Steel and the Corrosion Reaction
During the corrosion process, the steel will lose iron atoms into its environment in the form of ions. In return
some of the metal ions from the environment will plate out and return to the metallic state. This is known as
a reversible reaction. When the rates of the forward and reverse reactions are the same, then the process is
in equilibrium and the steel takes up its equilibrium potential.
Metal atoms leave the metal and they go into solution as positively charged metal ions, leaving behind
negatively charged electrons. Consequently, the metal becomes more negatively charged. This makes it
increasingly difficult or impossible for the remaining metal atoms to escape as positively charged ions as they
are being held by the negative charge of the metal.
For the process to continue, the excess of electrons in the metal must be consumed elsewhere in another
reaction. The manner and speed with which these excess electrons can be removed is one of the factors that
determine the rate of corrosion.
One important step in the corrosion of steel is the transformation of an iron atom to an iron ion by the loss of
two electrons. This is called the anodic reaction:
(1) Fe => Fe++ + 2e-
(IRON ATOM) => (IRON ION) + (2 ELECTRONS)
This reaction can only occur if there is a suitable electron acceptor to combine with the electrons released by
the ion atom. Freshwater or seawater contain dissolved atmospheric oxygen which readily serves this
The oxygen is electrochemically reduced to hydroxyl ions in the cathodic reaction.
(2) O2 + 2H2O + 4e- => 4OH-
(OXYGEN) + (WATER) + (4 ELECTRONS) => (HYDROXYL IONS)
The heterogeneous character of the metal surface allows for some areas or sites to favour reaction (1) and
become anodes and other areas to favour reaction (2) and become cathodes. The whole surface of the metal
is therefore divided up into large numbers of anodes and cathodes, as shown below.
Figure 1-1. Anodic & cathodic areas form on the uncoated steel surface.
As the anodic reaction can take place much more rapidly than the cathodic reaction most of the surface is
taken up with the production of hydroxyl ions, as shown in figure 1-2.
Figure 1-2. The cathode area is larger than the anode area on uncoated steel.
Figure 1-2 shows the progress of corrosion where metal is lost from the anode, causing it to progressively
become thinner, accompanied by a flow of electrons from the anode to the cathode which in turn react with
both oxygen and water from the environment to form hydroxyl ions.
Both the iron ions and the hydroxyl ions diffuse into the solution and then react together to produce ferrous
hydroxide as shown in reaction (3)
(3) Fe++ + 2OH- => Fe (OH)2
(FERROUS IONS) + (HYDROXYL IONS) => (FERROUS HYDROXIDE)
Ferrous hydroxide in the presence of an abundant supply of oxygen is oxidised to the familiar reddish brown
(4) 2Fe(OH)2 + O2 => Fe2O3.2H2O
(FERROUS HYDROXIDE) + (OXYGEN) => (RUST)
The above reactions, (1) (2) (3) & (4), are the basic reactions which occur when iron or steel transforms to rust
or, more specifically, to hydrated iron oxides. In practical situations the process is not so simple. For instance,
corrosion of steel in seawater or in polluted atmospheres results in more rapid and complicated reactions
producing corrosion products in association with iron oxide. Some of these iron salts are water-soluble and
can cause major problems to coatings if not removed before their application.
In given environments certain metals will form protective corrosion products, oxides that prevent or retard
further corrosion. Aluminium and stainless steel are examples of this.
Factors Influencing Corrosion Rates
In the majority of cases, the corrosion rates of metals are controlled by the diffusion of reactants to and from
the metal surface, hence freshly exposed bare steel surfaces will corrode at a greater rate than those covered
with a compact layer of rust.
The corrosion rate is also heavily controlled by the diffusion of oxygen through the water to the steel surface.
Areas where oxygen diffusion is easy will corrode the fastest.
Figure 1-3. Diffusion pathways in the corrosion reaction on uncoated steel.
High flow areas such as in the vicinity of bell mouths will tend to exhibit higher corrosion rates because of the
increased oxygen levels, although erosion is also a factor here.
Areas covered by a thin, conducting, moisture film, such as the conditions found in ballast tanks after the
ballast water is removed and the conditions in cargo tanks after sea water washing, will corrode faster than
areas under immersion. Therefore the ullage space at the top of ballast tanks and at the top of double bottom
tanks where air has become trapped, tend to corrode more quickly than deeply submerged areas where there
is a lower oxygen availability.
As corrosion rates are determined by diffusion, diffusion rates are also controlled by temperature. Steel and
other metals therefore corrode at faster rates at higher temperatures than at lower temperatures. As a result,
underdeck areas and regions adjacent to the engine room or to a hot cargo, will tend to corrode preferentially.
One of the features of the modern double hulled tanker with fully segregated ballast tanks, is that when the
cargo tanks are fully loaded, the empty ballast tanks act as a vacuum flask or thermo-bottle and retain the
heat in the cargo for significantly longer periods than the single hull design.
This increase in temperature of the cargo / ballast bulkhead combined with the cooler outer shell bulkhead (in
the underwater regions) produces a complex set of corrosion conditions and results a driving force which
increases the corrosion rate of the steel in the ballast tanks. Corrosion rates in the cargo tanks themselves will
also be higher due to the increased temperature.
For corrosion to occur, there must be a conductive medium between the two parts of the corrosion reaction.
Corrosion will not occur in distilled water and the rate of corrosion will increase as the conductivity increases
due to the presence of more ions in the solution.
The corrosion rate of steel reaches maximum close to the normal ionic content of sea water. Fresh water
corrodes steel to the least extent, then brackish or estuarine water, with sea water being the most corrosive
Type of Ions
Some types of ions present in seawater or in cargoes are more corrosive than others. Chloride ions are usually
the most destructive with sulphate and other sulphur containing ions also representing a major problem.
Chloride ions have a destructive effect on the protective properties of any rusts produced by preventing the
formation of the more protective, densely packed oxides. Sulphur containing ions become involved in
additional electron generating reactions within the rust itself which in turn forms a cyclic, self regenerating
process. This can produce intensive pitting on the inner bottoms of cargo tanks in oil and product carriers.
The sulphur can originate from both the inert gas system and from any sulphur containing cargoes such as
sour crude oil.
Acidity and Alkalinity (pH)
pH is a measure of the acidity or alkalinity on a scale of 1 to 14. pH 7 is neutral. In neutral seawater, the pH is
around 7.5 which means that the hydrogen ions (acid) and hydroxyl ions (alkali) are almost in balance. Under
such circumstances, the reaction that balances the iron dissolution is the reduction of dissolved oxygen to
form hydroxyl ions. If however the environment becomes more acid and the pH falls closer to zero, then there
is a greater quantity of hydrogen ions than hydroxyl ions present in the solution. The excess hydrogen ions
can become involved in the balancing (cathodic ) reaction which results in the evolution of hydrogen gas. As
both the hydrogen ions and the hydrogen gas can diffuse very rapidly, the steel can corrode very much faster.
This is a common effect when carrying cargoes such as petcoke, sulphur and sour crude oils.
Under alkaline conditions, where there is an excess of hydroxyl ions and the pH can increase towards 14, steel
cannot corrode by either mechanism and remains unattacked.
Many of the blisters which are found in ballast tanks, particularly in the double bottoms, are filled with a high
pH fluid. When the blister caps are removed, the steel is bright underneath. However, it will begin to corrode
once the cap is removed, so once one or two of a group of blisters have been checked and the liquid found to
be alkaline, the remainder of the blisters should be left intact.
Every metal takes up a specific electrochemical potential when immersed in a conducting liquid. This potential
is called the half cell potential as it can only be measured by comparing it to another known reference
potential produced by a reference electrode. Common reference electrodes are the Saturated Calomel
Electrode (SCE), silver/silver chloride and copper/copper sulphate reference electrodes.
The potential that a metal takes up in a solution can determine if and how fast it will corrode. The potential
can be changed by connecting it to another dissimilar metal (as in galvanic corrosion or by using sacrificial
anodes) or by applying an external potential, as occurs with an active cathodic protection system of the type
employed on the external hull.
Types of Corrosion
The most common type of corrosion encountered is the general attack of a more or less uniform nature,
although the loss of metal is concentrated at the anode sites and there is a continual change in the surface
with time. With progressive metal loss, areas which were initially anodic cease to be active and new anodic
sites take over. There is thus a continuous interchange between the anodic and cathodic areas, such that over
a period of time the loss of metal over the entire surface is fairly uniform.
This is the easiest form of corrosion to combat or allow for because structural life time can be predicted, a
feature which is not possible with the following corrosion forms.
The characteristic of this type of attack is that it is extremely localised and the penetration is deep in relation
to the area attacked. Pitting is one of the most dangerous forms of corrosion as it often occurs in places
where it cannot be readily seen. Pitting corrosion can be extremely intense on mill scale covered steel which
has been left outdoors and has weathered, as shown in the figure below.
Figure 1-4. Pitting corrosion on uncoated steel, showing layers of iron oxides.
Pitting corrosion can occur whenever there are suitable localised conditions. Typically pits form where there is
a small anodic area which is supported by a large cathodic area. In vessels this can occur at isolated areas
where the coating has been damaged. The corrosion occurs at the exposed steel area and the coating and the
steel under it become the cathodic area.
A ring of blisters surrounding an active anodic site are common, as shown in photograph 1-1.
Before segregated ballast tanks were introduced, cargo tanks with heating coils such as stainless steel, which
were also used as ballast tanks, pitted severely. This was due to galvanic corrosion.
Photograph 1-1. Cathodic blisters surrounding active anodic site.
On uncoated stainless steel pipe work, for example, pitting can occur where the passive oxide layer becomes
damaged and corrosion can initiate at individual sites. If the corrosion products are not washed away from
the surface, they will continue to cause corrosion and small pits will form. The materials needed for corrosion
become trapped in the bottom of the pits and the rate of corrosion can accelerate as the pit develops.
Pits can grow in a variety of shapes, the common ones are saucer, V shaped and under cut pits, as shown in
Figure 1-5. Different pit shapes.
V shaped pits tend to be the most serious of these four types of pitting, as the rate of penetration through the
steel can be very high. Once this type of pit becomes established, it is very difficult to clean the corrosion
products from the base of the pit and the corrosion rates can become very rapid.
Under cut pits are also a serious problem as the actual metal loss is greater than is initially apparent. If the
pits are relatively shallow, then the overhang area can break under pressure and the pits “open up”, losing the
aggressive contents to the environment.
Over a large area such as a tank top, the effect can be the equivalent of rapid general corrosion. If the pits do
not become open, then the rate of corrosion can increase as the pits contain all the constituents necessary for
corrosion and the anodic and cathodic areas can separate out within the pit. As with the V shaped pits, these
are extremely difficult to clean thoroughly and corrosion rates can be high.
Saucer shaped and stepped pits are the least detrimental, as the rate of metal penetration is relatively low
over short time periods as compared with the other types.
Intense localised corrosion, ranging from small pits to extensive attack over the whole surface, can occur
within narrow crevices formed by the geometry of a structure, for example: riveted plates or threaded joints.
Crevice corrosion is characterised by a geometrical configuration in which the cathode reactant, oxygen, can
readily gain access to the metal surface outside the crevice and less access to the crevice. The metal within
the crevice is therefore anodic to the surrounding steel and suffers preferential corrosion.
Figure 1-6. Crevice corrosion.
When mud, poorly adherent coating, sand and other debris cover a passive surface it undergoes a similar type
of attack to that occurring in crevices. Wherever loose debris collect, there will be a depletion of oxygen in a
crevice. Consequently, the attack is localised there.
Crevice corrosion and subsequent pitting can also initiate where particles of material such as soot fall on an
exposed metal surface. Crevices form where two surfaces are in close contact, for example pipes and pipe
support brackets in ballast and cargo tanks can suffer from crevice corrosion where the two items touch. If
they are constructed from different metals, one will tend to corrode preferentially. Where they are made
from the same metal, both may develop pits where they are in contact.
An example of crevice corrosion forming pits is shown in photograph 1-2.
Photograph 1-2. Pits forming as a result of crevice corrosion between U bolt and pipe.
In the galvanic series below the reference potential is a Standard Calomel Electrode (S.C.E.). This is a common
reference point in chloride containing environments such as are found in the marine industry. The figure
below gives the ranking of a number of common engineering materials in the Galvanic Series. The most
positive (noble) material will be protected against corrosion at the cost of the most negative (base) material.
Figure 1-7. The Galvanic Series of metals with the most noble (least easily corroded) at the bottom.
When two metals in the series are electrically in contact one of them becomes the anode in the corrosion
reaction and the other becomes the cathode. Anodes corrode in preference to cathodes. Cathodes will
normally be at the sites of the oxygen reduction reaction.
For instance when steel and copper are connected as in the diagram below, steel is the less noble and
therefore corrodes rapidly, whereas the copper is unaffected apart from its surface becoming more alkaline.
Figure 1-8. Flow of electrons in the iron – copper couple.
In accordance with the traditional concept, an electrical current travels from the copper to the steel (from the
positive cathode to the negative anode).
Corrosion of the steel is accelerated through its contact with copper. The steel suffers galvanic corrosion while
the copper is protected cathodically.
Microbiologically Influenced Corrosion (MIC)
This type of corrosion can very occasionally occur in ballast tanks and has sometimes been blamed for the
excessive pitting to be found on the tank tops of VLCC’s. All metals, even stainless steel, may incur corrosion
from microbiologically influenced corrosion. It is very difficult to clearly differentiate MIC definitively from
other forms of corrosion and opinions differ widely as to its significance. Only when mats or webs of slimy
material are present in clearly deoxygenated environments can its presence be definitively confirmed.
The two most common types of bacteria that cause corrosion are Acid Producing Bacteria (APB) and Sulphate
Reducing Bacteria (SRB). Both live in colonies attached to the surface of the steel where they assist each other
in their growth. Corrosive bacteria such as SRB which grow in oxygen free environments, rarely thrive over
large areas in the conditions on board vessels. On ships, microbes can live in the water layer at the bottom of
oil cargo tanks and in the sediment in ballast tanks, but stagnant conditions are usually required for MIC to
become wide spread. The exact reaction of microbes and steel is not very clear, but they do produce acids,
create corrosive cells & produce hydrogen sulphide
The initial detection of bacteria is first achieved visually by noting a black slime deposit on the surface of the
steel. Additionally, the detection of Hydrogen Sulphide (as a rotten egg smell) could possibly be noted.
Corrosion attributed to MIC is almost always highly localised pitting and the pits are generally filled with a
black ferrous product. The walls of the pit can be terraced and the metal surface below the corrosion
products is often bright and active. Further confirmation can be obtained by culturing samples.
However, similar effects can also be found where MIC is not a factor. In crude oil tanks, the corrosion and
pitting are driven mainly by sulphur deposits from the cargo or produced by inert gas systems.
All permitted hard coatings used in cargo and ballast tanks are known to be resistant to bacteria with the
possible exception of vinyls. The latter are only rarely used in these areas.
Supplementing a coating protection system with anodes can cause the pH within the tank to increase.
Bacteria do not usually thrive in areas where the pH level is in the alkaline range of 10 to 14.
Note that although sacrificial anodes may be present, the local pH under a biofilm or rust scale may become or
remain acidic, if it is shielded from the effects of the sacrificial anode.
The use of biocides for treating bacterially affected areas has been tested successfully in small, enclosed tanks,
but these have short time effects and are expensive. Biocides such as chlorine, hydrogen peroxide, iodine and
quaternary amine have been used.
At the new construction phase, design features should be utilised in eliminating areas for the accumulation of
mud and sediment. Also, proper drainage of all liquids to a common stripping area is desired to eliminate the
possibility of stagnant water accumulating. Good design is safe, environmentally acceptable and permanent.